INTERNATIONAL SCHOOL FOR ADVANCED STUDIES

CONDENSED MATTER THEORY SECTOR

### Molecular crystal structure prediction with

### evolutionary algorithm

Thesis submmitted for the degree of Doctor Philosophiæ Academic Year 2014/2015

CANDIDATE Cong Huy Pham

SUPERVISOR Prof. Stefano de Gironcoli

October 2015

## Contents

Contents 3

Introduction 5

1 Ab-initio Electronic Structure Calculation 11

1.1 Density Functional Theory. . . 12

1.2 GIPAW Method. . . 16

1.2.1 Projector-Augmented-Wave . . . 16

1.2.2 Gauge-Including Projector-Augmented-Wave . . . 18

2 Molecular crystal structure prediction with evolutionary algorithms 21 2.1 Introduction to atomic crystal structure prediction . . . 21

2.2 Introduction to molecular crystal structure prediction. . . 23

2.3 Challenges in crystal structure prediction of molecular crystal . . . . 24

2.3.1 The search space is huge . . . 24

2.3.2 Addressing the relative stability of polymorphs is dicult . . 25

2.4 Evolutionary algorithm in the case of molecular crystal . . . 26

2.4.1 Initialization . . . 27 2.4.2 Local optimization . . . 27 2.4.3 Selection. . . 29 2.4.4 Variation operators . . . 29 2.4.5 Convergence conditions . . . 30 2.4.6 Further notes . . . 30

3 Molecular crystal structure prediction of glycine 33 3.1 Introduction . . . 33

3.2 Method . . . 35

3.2.1 Evolutionary search . . . 35

3.2.3 Cluster analysis . . . 36

3.3 Results. . . 37

3.3.1 Performances of several van der Waals functionals . . . 37

3.3.2 Results of evolutionary algorithm . . . 40

3.3.3 Clustering algorithm . . . 42

3.3.4 Identication ofζ-glycine . . . 47

3.3.5 Challenges in exploring α-glycine . . . 48

3.3.6 Notes on the γ-glycine . . . 49

3.3.7 New low-energy structures of glycine . . . 50

3.4 Conclusion. . . 52

4 Molecular crystal structure prediction of cholesterol 57 4.1 Introduction . . . 57

4.2 The complexity of the energy-landscape of ChAl . . . 60

4.3 Method . . . 66

4.3.1 Evolutionary search . . . 66

4.3.2 ab initio calculations . . . 67

4.3.3 GIPAW calculations . . . 67

4.4 Results. . . 67

4.4.1 Results of evolutionary algorithm . . . 67

4.4.2 Validation of the classical force-eld . . . 68

4.4.3 Relations between levels of relaxation, structural properties and NMR spectra. . . 71

4.4.4 Identifying the experimental structure of ChAl . . . 74

4.4.5 Prediction of new structures of cholesterol and their NMR spectra. . . 75

4.5 Conclusion. . . 77

5 Summary and Outlook 79

A Detailed results of evolutionary algorithm searches for low-energy

Contents 5

## Introduction

Molecular polymorphism, the observation of dierent crystal structures made up of the same molecules, has been a central problem standing in the way of aordable and reliable crystal structure prediction which would greatly accelerate the devel-opment of new materials for applications in solid state chemistry, material science and pharmaceutical science [1]. In summary, the key challenges for ab initio crystal structure prediction of molecular crystals include i) the computational cost of ther-modynamical exploration of a rich polymorphic phase space; ii) the accuracy needed to resolve the similarly-low energies among polymorphs [2]; and iii) the fact that the crystallization procedure is controlled by kinetic factors rather than thermodynamic ones [3].The last decade has witnessed these challenges being tackled by the scientic community and the progress can be followed through the blind tests organized yearly by the Cambridge Crystallographic Data Centre [4,5,6,7,8]. The exponen-tial growth in the hardware performance and new, ecient algorithms tailored for molecular crystals have allowed a wider region of the phase space to be explored. The increased computational performance also enabled a transition from empirical interatomic potentials to more accurate but time consuming quantum mechanical techniques, mainly Density Functional Theory (DFT). However, this transition did not guarantee an increase in the predictive power in all cases [9]: the standard DFT functionals do not describe properly van der Waals (vdW) interactions. This fact forces crystal structure prediction studies to employ the approximate semi-empirical corrections. These approximations to the vdW interactions strongly aect the en-ergy ordering of the explored structures, which is a core information in predicting polymorphism. Hence, to render crystal structure prediction reliable, a fully ab initio method that is able to obtain an accurate lattice energy including the vdW interactions has been highly desirable.

Recently a breakthrough in the description of vdW interactions in DFT has been made: many new non-local functionals that accurately describe the dispersion

interactions have been proposed and demonstrated unprecedented success in a wide range of systems from molecules, molecular crystals to layered materials, with a computational cost comparable to that of standard functionals [10, 11]. Even in dicult cases such as glycine crystals, where polymorphs show energy dierences as little as 1 kcal/mol, new non-local functionals can yield the correct stability ordering as well as the accurate pressure evolution [12].

Encouraged by these results we combine this critical progress in DFT with recent developments in evolutionary crystal structure prediction [13], specically adapted for molecular structure search [9], and perform a fully ab initio crystal structure pre-diction search on glycine crystals, without semi empirical corrections in the energy description, using neither information on cell geometry nor the symmetry of the experimentally observed polymorphs. Thus it gives us the right to assess whether state-of-the-art ab initio crystal structure prediction can pass the challenging blind test of exploring the phase space of polymorphic glycine. In this study, we obtain, without prior empirical input, all known phases of glycine, as well as the structure of the previously unresolvedζ phase after a decade of its experimental observation [14].

The search for the well-establishedαphase instead reveals the remaining challenges

in exploring a polymorphic landscape. We also propose several low-energy structures of glycine, some of which are more stable than the experimental structures.

The study of crystal structure prediction for cholesterol is motivated by a med-ical application: a solid state nuclear magnetic resonance experiment reports that dierent pathologies of human gallbladder result in cholesterol gallstones with dier-ent polymorphs [15]. These polymorphs show distinct nuclear magnetic resonance (NMR) spectra and a phase which associates to gallbladder cancer, has not been structurally determined yet. Important information on the growth of gallstones associated to dierent diseases can be revealed if the crystal structure of the un-known phase is identied. In this work, we use evolutionary algorithm in the case of molecular crystal in the USPEX code [9] combined with a classical force-eld. This force-eld was designed specically for cholesterol and its success in determin-ing the crystal structure of cholesterol polymorphs has been reported [16]. Later in our study we discuss the validation of the classical force eld as a primary selection

Contents 9 method. After using accurate DFT calculations within non-local van der Waals functional the lowest energy predicted structure is identied with the experimental one based on their good agreements for crystal structure parameters as well as NMR spectra. We also propose a few low-energy structures of cholesterol and characterize them by their NMR spectra.

The layout of the thesis is as follow: In Chapter 1, we present the theoreti-cal background of DFT, Projector-Augmented-Wave (PAW) and Gauge-Including Projector-Augmented-Wave (GIPAW) methods. In Chapter 2, we introduce the crystal structure prediction problem and present evolutionary algorithms as one so-lution to perform crystal structure search for molecular crystals. Chapter 3 and Chapter 4 are dedicated to the detailed results when using evolutionary algorithm in crystal structure search for the studies of glycine and cholesterol respectively.

### Chapter 1

## Ab-initio Electronic Structure

## Calculation

From the theoretical point of view, in order to understand the properties of any system, all one needs to know is its wavefunction. It does not represent any physical quantity but at any given time, its square modulus is interpreted as the probability density of nding a particle at a given point in space. If the wavefunction is known, other observable quantities are easily calculated and the system is well-understood. This wavefunction is the solution of the well-known Schrödinger equation with the general form of the Hamiltonian

H=−X
i
~2
2m5
2
i−
X
α
~2
2Mα
52_{α}+1
2
X
i6=j
e2
|ri−rj|+
1
2
X
α6=β
ZαZβe2
|Rα−Rβ|
−X
i,α
Zαe2
|ri−Rα|,
(1.1)
where {ri} and {Rα} are the Cartesian coordinates of electrons and nuclei. The
rst (second) term is the kinetic energy of the electrons (nuclei) while the third and
fourth terms are the Coulomb interactions between electrons and nuclei, respectively.
The nal term corresponds to the electron-nucleus attraction.

In general, because of the large number of independent variables (growing with the number of electrons and nuclei), the exact solution to this equation can not be found. Fortunately, since electrons and nuclei are very dierent, one can treat them separately in the Born-Oppenheimer (or adiabatic) approximation [17, 18]. The physical basis of this approximation comes from the fact that electron mass is much smaller than the nuclear one. Therefore the electronic time scale is much shorter than the nuclear one and a good approximation can be obtained by keeping the nuclei xed and determining the ground state of electrons as a function of

static nuclear positions. Within this approximation, one just needs to solve the
Schrödinger equation for the electrons with the Hamiltonian that reduces to the
three terms
H=−X
i
~2
2mi
52_{i} +1
2
X
i6=j
e2
|r_{i}−rj|
−X
i,α
Zαe2
|r_{i}−Rα|
. (1.2)

However, even with this simplication, the problem for electrons remains too compli-cated and still is a many-body problem. Solving it is the main task of computational electronic structure.

In 1964, a breakthrough was made by Hohenberg and Kohn [19] in which the problem is simplied using density functional theory (DFT). The main advantage of DFT with respect to wavefunction methods is the use of electronic charge density as a fundamental variable, therefore greatly reducing the number of variables in the calculation.

### 1.1 Density Functional Theory

Hohenberg and Kohn have proven two theorems that are the basis for DFT [18,19]. The rst theorem states, For any system of interacting particles in an external potential Vext(r), the potential is determined uniquely, except for a constant, by

the ground state particle densityn0(r). Since the ground state density determines

the external potential Vext(r) and so the Hamiltonian for a given system, it follows

that the wavefunctions of all states (ground-states and excited-ones) are determined. Thus in general, all properties of the system are completely determined given only the ground state density. Mathematically, any property of a many-body interacting particles can be viewed as a functional of the ground state density. The total energy now reads

E[n(r)] =T[n(r)] +Uee[n(r)] +Uext[n(r)] =F[n(r)] + Z

Vext(r)n(r)dr, (1.3)

whereUext[n(r)] =R Vext(r)n(r)dr is the interaction energy of the electrons with an

external eld Vext(r),T[n(r)]andUee[n(r)]are the kinetic energy and the electron-electron interaction energy respectively. SinceF[n(r)] =T[n(r)] +Uee[n(r)]requires

1.1. Density Functional Theory 13 no explicit knowledge of Vext(r), it is an universal functional of the density (only

in the meaning that it does not depend on the external eld). The second theorem states that: the ground state energy is a functional of n0(r) and satises a

varia-tional principle, i.en0(r) minimizes the total energy E[n(r)]. The consequences of

the Hohenberg-Kohn theorems lead to a considerable conceptual advance. If the universal functional F[n] is known, one can nd the ground state electronic

den-sity for any system. Unfortunately those theorems give no information about this functional.

In 1965, Kohn and Sham developed a good approximation for the functional

F[n] by introducing an auxiliary non-interacting electron system which has the

same ground state density as the interacting one [18, 20]. With this assumption, the interacting electron problem is mapped onto an equivalent non-interacting one which is easier to solve. In this way, the functionalF[n]can be written as

F[n] =Ts[n] + 1 2 Z n(r)n(r') |r−r'| drdr'+Exc[n], (1.4) where the rst termTs[n]is the independent particle kinetic energy, the second one is the classical Coulomb interaction energy of the electron densityn(r)(the Hartree

energy). The last one is the exchange-correlation energy Excthat can be written as

Exc[n] =T[n]−Ts[n] +Uee[n]−

1 2

Z _{n}_{(}r_{)}_{n}_{(}r'_{)}

|r−r'| drdr'. (1.5) In this form, one can see that all many-body eects are included inExc. Remember that one needs to require the integration of the density giving the correct number of electrons R

n(r)dr = N. Minimizing the energy functional E[n], given in eq.

(1.3), with this constraint is equivalent to solve a set of self-consistent Kohn-Sham
equations
−1
2 5
2_{+}_{V}
KS(r)−εi
ψi(r) = 0,
VKS(r) = Vext(r) +VH(r) +Vxc(r),
VH(r) =
Z _{n}_{(}r'_{)}
|r−r'|dr', Vxc(r) =
δExc[n(r)]
δn(r) ,
n(r) = X
i∈occ
|ψi(r)|2. (1.6)

This is a nonlinear self-consistent system of equations because the Kohn-Sham po-tential VKS(r) depends on the solutions {ψi}. If the functional Exc[n] is explic-itly dened, the Kohn-Sham equations can be solved self-consistently by numerical methods.

So far DFT has been presented as a formal mathematical framework for view-ing electronic structure from the perspective of the electron density. The major problem is that the exact functionals for exchange and correlation are unknown, but approximations can be introduced to permit quite accurate calculations. These approximations have to reect the physics of electronic structure and do not come from the mathematical properties of DFT.

The simplest approximation for the exchange-correlation functional is the Local Density Approximation (LDA) which has a quasilocal form

E_{xc}LDA[n(r)] =
Z

εxc(r; [n(˜r)])n(r)dr, (1.7) whereεxc(r; [n(˜r)])represents the exchange-correlation energy per particle at point r. The idea of LDA is that for regions where the charge density varies slowly, the exchange correlation energy can be considered the same as that of a locally uniform electron gas of the same charge density. In practical use of LDA, the exchange term takes the simple analytic form for the homogeneous electron gas while the correlation energy is parameterized from accurate Quantum Monte Carlo data [21]. A typical limitation of LDA is that it underestimates ionisation energies but overestimates the binding energies. LDA also gives inaccurate descriptions for strongly correlated systems.

The Generalized Gradient Approximations (GGAs) are semilocal and take into account the gradient of the density at the same point

E_{xc}GGA[n(r),∇n(r)] =
Z

εxc(n(r),∇n(r))n(r)dr, (1.8) which in many cases improve on LDA, especially for cohesive and dissociation en-ergies. The rst GGA functional was introduced by Perdew and Wang in 1992 [22]. Many dierent forms of GGA functionals were proposed and the most widely use till now is named PBE from Perdew, Burke and Ernzerhof [23].

1.1. Density Functional Theory 15 It is well known that the lack of dispersion force is one of the biggest challenges of standard approximate DFT. The van der Waals interaction energy depends on atoms separationRasEvdW∝R−6[24] and neither LDA nor GGA can describe this

behavior correctly. In LDA, long-range interactions are described by an exponential decay whereas GGA makes corrections to the local approximation of LDA but is still unable to describe the van der Waals interaction behavior.

In recent years, many approaches have been proposed to deal with van der Waals interactions. Calculations using exact-exchange (EXX) and random-phase ap-proximation (RPA)-correlation energies within the adiabatic connection uctuation-dissipation theorem formalism have demonstrated to describe correctly the long-range van der Waals interaction [25,26,27]. Unfortunately, its high computational cost limits its practical use. A simple idea to account for van der Waals interactions is to add an empirical dispersion-energy term to the total DFT energy. Several meth-ods using this idea have been introduced, for example DFT-D2 [28], DFT-D3 [29] of Grimme et al., and vdW-TS of Tkatchenko and Scheer [30]. These methods need some predetermined input parameters to calculate the van der Waals interaction. Their limitation is that the complex many-body interactions are treated outside the DFT framework and therefore the ground state wavefunction and ground state density do not contain non-local correlation eects.

In other approaches, termed non-local correlation functionals, the dispersion interaction is obtained directly from the electron density. In these approaches, a non-local correlation term

E_{c}nl=
Z Z

dr1dr2n(r1)n(r2)φ(n(r1), n(r2),|r1−r2|), (1.9)

is included in the correlation functionals [10]. In eq. (1.9), n(r) is the electron

density and φ(n(r1), n(r2),|r1−r2|) is the integration kernel with a 1/|r1−r2|6

asymptotic behavior. The computational cost of the original formulation is quite demanding, especially in a plane-wave approach. Only after Román-Pérez and Soler [31] proposed an interpolation scheme to improve the scaling, these non-local func-tionals are widely used. Several non-local funcfunc-tionals were suggested and promising results have been obtained. In the original vdW-DF functional, revPBE functional

is applied for the exchange part [32]. Some other functionals are the same as vdW-DF except that other exchange functionals are employed instead of the revPBE, for example optB88-vdW and optB86b-vdW [33], c09-vdW [34], cx-vdW [35]. A second version of vdW-DF functional, named vdW-DF2 [36], with modied exchange and non-local correlation was suggested to improve the descriptions of the binding energy and equilibrium spacings between weakly-bound complexes. The VV10 functional [11] proposes a dierent functional form for the kernelφ(n(r1), n(r2),|r1−r2|)and

can depict accurate interaction energies of van der Waals system, not only near the minima but also far from equilibrium. It also gives accurate covalent bond lengths and atomization energies. Its revised version, known as rVV10 [37], allows the use of the Román-Pérez and Soler scheme and therefore makes the computation less expensive while keeping the outstanding precision of the original VV10. Recently, it was found that changing thebparameter of the rVV10 functional (from its original

value 6.3 to 9.3) gives a better description of structural properties in rst-principles molecular dynamics of liquid water [38].

In this thesis, we use the vdW-DF functional in studies of glycine and cholesterol. In the case of glycine polymorphs at ambient condition, the performances of rVV10 and rVV10-b9.3 functionals are also given for comparison.

### 1.2 GIPAW Method

The main concern of this thesis is crystal structure prediction. Moreover, in the study of cholesterol, we also characterize the predicted structures by their NMR spectra using the GIPAW method. In this section, we introduce very briey the Projector-Augmented-Wave (PAW) and Gauge-Including Projector-Augmented-Wave (GIPAW) methods. The details of these methods can be found in the original papers [39,40,41].

1.2.1 Projector-Augmented-Wave

One problem of DFT is the behavior of the Kohn-Sham one electron wavefunction. This wavefunction is fairly smooth in the bonding regions far from the nuclei whereas

1.2. GIPAW Method 17 close to the nuclei, because of the large electron-nuclear Coulomb attraction, it has rapid oscillations. For solving Kohn-Sham equation in a plane-wave basis set, this behavior requires a very large set to describe the wavefunction accurately.

The use of pseudopotentials is one way to overcome this problem [42]. Since the shape of the wavefunction in the vicinity of the nuclei does not aect much the electronic properties of the material, the rapidly oscillating wavefunction can be replaced by a smoother function. However, because of the way the pseudopotential is constructed, the information about the full wavefunction close to the nuclei is lost. As a result, the pseudopotential method cannot describe correctly properties that depend directly on the core electrons (such as X-ray photoelectron spectroscopy) or the electron density near the nuclei (such as NMR shielding and coupling constant). In another approach, namely augmented plane-wave (APW) method [43, 44], one also divides the space into two regions. Inside the atom-centered augmentation spheres, the wavefunctions are expanded in atom-like partial waves. In the bonding region outside these spheres, some smooth envelope functions are used. At the boundary of the spheres, the partial waves and envelope functions are matched.

The projector-augmented wave (PAW) method [39] is a generalization of the pseudopotential and APW ones. Its idea is that all-electron Koln-Sham single par-ticle wavefunctions |ψi can be built from the ctitious pseudo wavefunctions |ψ˜i through a linear transformation operator T. Since |ψ˜i and |ψi dier only in the regions close to the nuclei,T can be written as T = 1 +P

RTˆR, whereTˆR is

non-zero only within some spherical augmentation region ΩR enclosing the atoms. The transformation operatorT can be dened as

T = 1 +X
Rn
|φRni − |φ˜Rni
hpRn|, (1.10)
where n refers to atomic-state quantum numbers; |φRni and |φ˜Rni are the
all-electron partial waves and pseudo partial waves, respectively; |pRni are projector
functions (which are localized in the region ΩR) satisfying the orthonormal
con-ditions: hpRn|φ˜R0_{m}i = δ_{RR}0δ_{mn}. In this representation, all-electron operators are

quasilo-cal operators, the pseudo-operators can be written as ˜ A= ˆA+ X R,n,m |pRni hφRn|Aˆ|φRmi − hφ˜Rn|Aˆ|φ˜Rmi hpRm|. (1.11) The advantage of PAW method is that all-electron observable quantities can be calculated using the pseudo wavefunctions without the need to explicitly store all-electron wavefunctions in memory. This is important for the calculation of properties that directly depend on the core electrons or the electron density near the nuclei such as NMR.

1.2.2 Gauge-Including Projector-Augmented-Wave

It is known that nuclei that have spin one-half (for example 1_{H,} 13_{C ...) can have}

two possible spin states (which are degenerate) with magnetic quantum numbers

mS=±1/2. If the nucleus is placed in an external magnetic eldB, the interaction between the nuclear magnetic moment and the external eld determines an energy dierence between the two states ∆E =γ~|B|, where γ is the gyromagnetic ratio

that depends on the nuclear mass and charge. Since the two states no longer have the same energy, transition between spin states can be induced. This phenomenon is known as Larmor precession with the so-called Larmor frequency being ω0 = ∆E/~=γ|B|.

Consequently, one can expect that all nuclei of the same nuclear mass (which have the same γ) would have very similar NMR frequency since the frequency

de-pends only on γ and the magnetic eld B. However, this is not the case. In fact, the core and valence electrons also interact with the magnetic eld and contribute a shielding eect to the NMR frequency. Therefore one observes dierent frequen-cies for dierent nuclei depending on their chemical environment. This shift in the NMR frequency is called NMR chemical shift.

The chemical shielding tensor is determined as

Bin=−−→σ(r)B, (1.12)

where Bin is the induced magnetic eld. This magnetic eld is generated by the

1.2. GIPAW Method 19 be calculated as Bin= 1 c Z dr0 j(1)(r0)× r−r 0 |r−r0|3, (1.13)

where j(1) is the rst-order induced electric current. From this formula, it is clear that the calculation of the induced magnetic eld requires an accurate description of the induced current close to the nucleus. Therefore the PAW formalism is needed to reconstruct the wavefunction behavior close to the nuclei.

It is known that, in an uniform magnetic eld, a eld-dependent phase factor is created in any wavefunction when translating the whole system by a vector t

hr|ψ_{n}0i= exp[(i/2c)r.t×B]hr−t|ψni. (1.14)
A diculty of the PAW method, when applied to systems in magnetic eld, is that a
huge number of projectors would be needed to describe this wavefunction correctly.
The use of a eld-dependent transformation operator

TB = 1 + X Rn exp[(i/2c)r.R×B] |φRni − |φ˜Rni hpRn| exp[−(i/2c)r.R×B] (1.15) can solve this problem. This transformation operator denes a new method which is called gauge-including projector-augmented-wave (GIPAW).

The details of GIPAW method can be found in the original papers [40,41] and can be schematized as follows

|ψ(0)i → |ψ(1)i →j(1)(r0)→Bin. (1.16)

First one determines the eigenstate |ψ(0)i of the unperturbed Hamiltonian in the absence of the magnetic eld then calculates its linear variation |ψ(1)i. The rst-order induced electric current can be written as the sum of three terms, a bare contribution, a paramagnetic operator and a diamagnetic one. Next step is to obtain the induced magnetic eld Bin using eq. (1.13) and the shielding tensor −→σ

arcording to eq. (1.12). Finally the isotropic chemical shielding is given by its trace:

### Chapter 2

## Molecular crystal structure

## prediction with evolutionary

## algorithms

In this chapter, we will briey introduce the crystal structure prediction problem and describe the challenges in crystal structure prediction of molecular crystals. We then present evolutionary algorithms as one solution to perform crystal structure search for molecular crystals. The detailed applications of evolutionary algorithm and their results in the search for low-energy structures of glycine and cholesterol are given in Chapter 3and Chapter 4 respectively.

### 2.1 Introduction to atomic crystal structure prediction

Crystal structure is one of the most important information about a system since it determines material properties. Dierent arrangements of even the same atoms can result in completely dierent properties of the material. For example, graphite and diamond are both made of carbon atoms but with dierent structures. In graphite, the atoms stay in layers with a hexagonal lattice while diamond has a tetrahedral form. In term of properties, graphite is a dark, soft material and is a good electrical conductor while diamond is transparent, the hardest material known up to now, and is an insulator. Thanks to the development of computational simulations, one can now determine a huge number of interesting properties of materials, assuming that their crystal structure is known. But if the crystal structure is unknown, one can gain very little information about the material.

Crystal structure is usually determined using experimental data from single-crystal X-ray Diraction (XRD) and/or NMR spectra. Unfortunately, in many cases, the quality of the experimental data is poor, for example at some experimental conditions of high pressures and/or high temperatures; and the positions of hydrogen atoms are not measurable in standard XRD experiments. In these cases, crystal structure prediction has a leading role in the determination of the crystal structure of the material. Crystal structure prediction is also a good approach to investigate materials at extreme conditions (e.g ultrahigh pressure) that cannot or are dicult to be studied with today's experimental techniques. In searching for new materials, computational crystal structure prediction is usually much easier and cheaper than experiments.

There is no doubt that crystal structure prediction is extremely challenging and it was even stated that crystal structures are unpredictable [45,46]. The main task in crystal structure prediction is to nd the global minimum in a multi-dimensional space. For a structure withN atoms in the unit-cell, the dimensionality of the space

is 3N + 3 (3N −3 for the atomic coordinates plus6 for the unit-cell parameters).

This space is huge and noisy with the number of possible structures increasing exponentially with the number of atoms in the unit-cell. Until now there is no method that can guarantee to nd the global minimum successfully.

Several methods have been proposed to overcome the diculty of searching a complex energy-landscape: data mining [47], metadynamic [48,49], basin hopping [50], simulated annealing [51,52] minima hopping [53] and evolutionary algorithms [13]. All of them work based on the assumption that one needs to explore only the most promising regions in a huge energy-landscape. The idea of data mining is simple: one has databases that contain a huge number of known crystal structures; in order to nd the structure of a new material, one can search in the databases the structures which have chemical composition similar to the one of the system that one wants to study. Then ionic substitutions are used and the structures are optimized with the expectation that the lowest energy structure found will be the ground state one. In metadynamic, basin hopping, simulated annealing and minima hopping methods, one starts from an initial structure which can be chosen in a

2.2. Introduction to molecular crystal structure prediction 23 good region of the energy-landscape. and then modies it by some perturbations in the cell parameters and/or atom coordinates. The optimization is performed with the hope that the structure will move to a new local minima. The scheme of evolutionary algorithms will be presented in the Section 2.4.

The so-called random sampling method in principle can explore many regions of the energy-landscape. The idea of this method is that candidate structures are created randomly and local optimization are performed for these structures. The search is then terminated when the lowest energy structure has been found several times. This method has been used for predicting crystal structure of some sim-ple systems and the results were very promising. However this method can work eciently for small systems up to around 12 atoms only [54].

### 2.2 Introduction to molecular crystal structure

### predic-tion

Prediction of the crystal structure at the molecular level is essential since molecular crystal can be used in many elds such as pharmaceuticals, optoelectronic materials, pigments, explosives, molecular electronics and metal-organic frameworks [3, 55]. In general, dierent polymorphic forms of a certain compound have signicantly dierent properties. Therefore in order to understand the properties of molecular crystals for industrial applications, knowing the molecular crystal structures and the condition at which they are stable is compulsory. To obtain the phase diagram of a molecular crystal, it requires the calculation of nite-temperature thermodynamic contributions and the understanding of the competition between thermodynamics and kinetics in packing determination. These issues are beyond the aim of this thesis. In this study, we only focus on nding the most thermodynamically stable molecular arrangements at 0 K.

The traditional way to do crystal structure prediction for molecular crystal is to rst rank the energies of all generated structures using classical force-eld. Those structures are created randomly from a given molecular conformations. The num-ber of generated structures may be as huge as 107 and the force-eld rules out a

signicant number of the worse structures. Then accurate DFT calculations are used to estimate the stability of all the short-listed candidate structures. There are several global optimization algorithms that can be extended from simple atomic crystal structure prediction to search for molecular crystal structure. Promising re-sults have been obtained by several studies using, for example metadynamic [56,57], minima hopping [58,59] and evolutionary algorithms [9,60,56].

### 2.3 Challenges in crystal structure prediction of

### molec-ular crystal

When doing crystal structure prediction for molecular crystals, an important aspect must be noticed. In general, the molecular crystal of certain molecule is thermo-dynamically less stable than the individual simple molecules that can be obtained from the chemical decomposition of the molecule of interest. For example, glycine (C2H5NO2) polymorphs maybe less stable than the combinations of H2O, CO2, CH4, NH3, H2, N2, NO2... Therefore in order to search for the crystal structure

of molecular crystals, it is a good idea to x the intramolecular connectivity of the molecule. It is not a limitation but in fact an advantage that reduces the search space and the number of degrees of freedom in the system.

Even when the whole molecule is used as the unit, the crystal structure prediction of molecular crystals remains dicult. The key challenges for ab initio crystal structure prediction of molecular crystals can be summarized as: i) the search space is huge; ii) addressing the relative stability of polymorphs is dicult.

2.3.1 The search space is huge

In molecular crystals, each molecule in the unit-cell is characterized by the coor-dinates of the molecule center and the angles of its orientation. In principle, for a certain number of a given molecule, there is an innite number of possible structures that can be formed. Among them, only the ones with lowest energies (or enthalpies if non-zero pressure is considered) are likely to be found experimentally. Predicting the lowest energy structures in such a huge energy-landscape is a big challenge.

2.3. Challenges in crystal structure prediction of molecular crystal 25 For exible molecules, there are usually more than one inequivalent molecules in the unit-cell. In this case, the number of degrees of freedom becomes even larger; and it is a good idea to use several types of molecules to describe possible dierent conformations [61,62]. We will do so in the study of cholesterol molecule which has a exible hydrocarbon tail.

The development of crystal structure prediction methods is aimed at making the search in the energy-landscape more ecient. Although several searching algorithms have been proposed with encouraging results [58, 59, 9, 60], currently there is no single method that can prove to address the general global minimum search success-fully. For the lowest energy structure found by any algorithms, there is no way to know if it really is the ground state structure or just a local minima. What one can do is to compare the lowest energy structures with the available experimental data. 2.3.2 Addressing the relative stability of polymorphs is dicult All structures created by crystal structure prediction methods need to be optimized to estimate their energies (or enthalpy if at non-zero pressure). The lowest energy structure found is assumed to be the ground state one. There is no doubt that predicting the right energy ordering is a prerequisite to nd the global minimum successfully.

In comparison with the atomic crystal, molecular crystal structure prediction is more challenging because of the accuracy needed to resolve similarly low energies among polymorphs. In molecular crystals the molecules are held together by van der Waals interactions and the energy dierences between structures are small. In some cases these energy dierences are even smaller than the typical numerical error of the simulation. Therefore a good treatment of long-range dispersion interactions is deeply needed.

Many crystal structure prediction studies for molecular crystal use classical force-eld as the local optimization due to its favorable computational cost compared with DFT calculations in quantum chemistry. Unfortunately, empirical potential energy-landscape often gives unphysical minima [63,64]. Inaccurate force-eld parameter-ization can lead to signicant distortion of the molecule and wrong energy ranking

of the candidate structures. Flexible molecules not only add more complexity in the energy-landscape but also make the accuracy of classical force-eld become more uncertain. It is known that there is usually considerable noise that may give rise to many local minima in the hypersurface of the force-eld. Structures that are optimized with this force-eld may be trapped in these local minima [61].

### 2.4 Evolutionary algorithm in the case of molecular

### crys-tal

Evolutionary algorithm is one of the methods that are well suited for structure pre-diction. It requires very little information as input. For molecular crystal structure prediction, only the molecular geometry and the number of molecules in the unit-cell are needed. The evolutionary algorithm works based on the idea of natural competi-tion and the survival of the ttest. Its scheme, as implemented in the USPEX code for molecular crystal, is sketched in Fig.2.1(a) and summarized in the following

Figure 2.1: (a) The scheme of evolutionary algorithm for predicting crystal structure of molecular crystal with the sequence of the steps that are performed; (b) sketch of how heredity, coordinate mutation and rotational mutation operators create a child structure: heredity combines slices of two parent structures in a new structure; co-ordinate mutation moves some molecules in a random direction; rotational mutation rotates the molecules by a random angle. This picture is reproduced from Ref. [9].

2.4. Evolutionary algorithm in the case of molecular crystal 27 2.4.1 Initialization

First, the code starts with some initial structures that are usually created randomly from an unit which is the whole molecule, instead of individual atoms as in the case of atomic crystal. The diversity of this generation guarantees the success of the search. In the USPEX code, instead of putting molecules at completely random positions, the structures are built from a space group that is chosen randomly. Experience shows that by doing so, the rst generation is proved to get higher diversity [9].

For large systems with a huge volume and a huge number of molecules in the unit-cell, the randomly generated structures are very similar to a disordered system and the unit-cell splitting technique [65] could be used. The large cell is split into subcells which contain smaller number of molecules. In the subcell, the molecules are placed randomly. This technique was shown to produce more diverse structures for large systems [65].

Some constraints can be applied at this initial step. One may need to set a min-imum distance between molecules to avoid molecules overlap. If any experimental information (cell parameters or crystal structure space group symmetry) is known, it can be used to make the search more ecient. If any structure is already known (from the studied compound or other related materials) it can also be included as template in the USPEX code (the Seed technique).

The use of space group information can be of great help in crystal structure prediction [66]. From the experimental organic crystal structure database, known crystals mostly belong toP21/c,P1,P212121,C2/c,P21andP bcaspace groups. In

the study of glycine, we will show that the use of this information allows to explore the energy-landscape more eciently.

2.4.2 Local optimization

At any generation, the created structures need to be optimized. The optimization process not only gives an estimate of the energy of the candidate structures in order to nd the lowest ones but also reduces the dimensionality of the energy-landscape. In some cases, structures that look very dierent at the beginning become the same

after relaxing with dierences just due to numerical noise.

Using accurate DFT in the local optimization would be a very desirable option. The advantage of ab initio calculations over the empirical force-eld ones is that ab initio can give accurate results in all regions of the energy-landscape while the

results of force-eld are good only near the regions where force-eld parameters were tted. Therefore ab initio calculations can be used in the study of new materials

where no experimental data are known. However insuciently dense k-point

sam-pling and/or bad pseudopotentials can produce inaccurate minima [54] and since molecules interact with each others by van der Waals interactions, the functional used must include this long-range interaction. In the study of glycine, we use DFT calculation in the local optimization and the vdW-DF functional [10,32], which pre-dicts correct energy ordering for simple organic crystals [12]. The k-point sampling

and pseudopotentials are carefully checked.

When the number of atoms in the unit-cell is large, the use of DFT in the local optimization step is too demanding and the use of classical force-eld is needed. In this case a good force-eld is required. Great improvements of the force-eld have been made so far. The all-atom force-eld is usually parameterized from DFT calculations in which dispersion interaction is included. Excellent agreements with experiments and/or quantum mechanical calculations have been achieved, even for exible molecules [61, 67, 62]. Indeed if the force-eld can be designed correctly, they are much appropriated for crystal structure prediction [4, 5, 6, 7, 8]. In the study of cholesterol, we will use a classical force-eld in the local optimization, whose successful determination of the crystal structure of cholesterol polymorphs has been reported [16]. Good candidate structures are then relaxed better using accurate DFT calculations with non-local van der Waals functional. One thing must be noticed as mentioned in Ref. [61]. Even a good force-eld may still have a noisy energy hypersurface, therefore with a good force-eld, the best strategy is to optimize the structure three times: rst step is done with the force-eld in the crystal structure prediction search; the obtained structures are then relaxed with an accurate DFT method; and nal one is relaxed with the force-eld again. If the latter optimization with force-eld produces a lower energy than the previous one,

2.4. Evolutionary algorithm in the case of molecular crystal 29 the structure has escaped a local minima. We will also do this check.

2.4.3 Selection

It can happen that in one generation, one structure is found many times and the same parent structures are likely to create very similar children. Therefore if a repeated structure is included when choosing parents structures for the next gen-eration, this may result in a waste of resource in the repeated optimization of the same structure. This duplication also reduces the diversity of the generation and makes it dicult for the algorithm to escape from local minima.

It is non-trivial to identify equivalent structures since there are many ways to represent a structure and numerical noise makes the problem more complicated. In principle one can not distinguish structures from their energy and volume alone [68]. In the USPEX code, the structures are classied by comparing their ngerprints. This function is related to the radial distribution function and diraction spectrum. Details of the ngerprint function in USPEX are given in Ref. [69, 70]. There is a technical issue when calculating the ngerprint for molecular crystals. The intramolecular contributions, which are the same for all molecules with dierent orientation, are neglected [9]. The molecule is then treated as a single object with the coordinates of the molecular center.

Based on the desired property, dierent selection rules can be applied: if one looks for the most stable structure then all the structures are ranked by their energy. The worst structures with highest energy are discarded and the lowest ones are likely to be chosen as parents to create the new generation.

2.4.4 Variation operators

When the parent structures are selected, the children ones are created by applying some variation operators. Some operators are shown in Fig2.1(b). Typically it is a good idea to keep some of the best structures from the previous generation to make sure that the generations don't go worse. These best structures are required to have signicantly dierent ngerprints. For coordinate mutation operator, the

molecules are moved in random directions and the rotational mutation operator chooses to rotate a certain number of molecules by a random angle. More details about mutation operators can be found in the original paper [9]. The diversity of the population is guaranteed by adding new random structures at each generation. Heredity operator is an essential part of the evolutionary algorithm. Without it, evolutionary algorithm becomes very similar to other random search methods. For other operators, the child structure is created from one single parent while for hered-ity, two structures act as parents. The heredity operator cuts planar slices from the two parents structures and combine them together to generate a child structure. One thing must be noticed in this case: if two good parents are very dierent the child structure can be very bad [71]. The reason is that the child structure falls into the high barrier region between two good local minima. In order to avoid this, in USPEX, the parents for heredity operators must have ngerprints that are not too dierent.

2.4.5 Convergence conditions

At each generation, the conditions for the convergence predened by the user are checked. One may want to stop the calculation when it reaches a specied maximum number of generations, or when after a given number of consecutive generations, no better structures are found. The later condition is inspired by the fact that at a certain generation, if no better structure is found, the parents would be the same as in the previous one and therefore the generation has more chance to be repeated. 2.4.6 Further notes

In the evolutionary algorithm, several parameters can have an impact on the eec-tiveness of the search. One has to deal with incompatible requests: the diversity of the population and the convergence to the optimal solution. With higher diversity, one can explore the energy-landscape better however the chances to search in the most promising regions are lower. On the other hand, reducing diversity helps to investigate a given region but increases the risk of missing the global optimum. In

2.4. Evolutionary algorithm in the case of molecular crystal 31 general, one seeks for a balance between diversity and convergence. Detailed study about this aspect can be found in Ref. [72].

There are advantages and disadvantages in evolutionary algorithms over other crystal structure prediction methods. The power of evolutionary algorithms is that they don't require previous system knowledge (except its chemical composition), which is good for the prediction of new materials. In each generation, the best structures are selected to procreate and, through new generations, increasingly better structures are found. However, in evolutionary algorithms, no information on mechanisms of phase formation is given. This information can be found from other methods, for example metadynamic [48, 49], basin hopping [50], simulated annealing [51, 52] and minima hopping [53]. While phase transition mechanisms can be simulated with such methods, real mechanisms present in experiments can be much more complicated and dicult to treat. Comparison of evolutionary algorithm with metadynamic and minima hopping can be found in Ref. [56] and Ref. [73,74] respectively.

### Chapter 3

## Molecular crystal structure

## prediction of glycine

In this chapter, we tackle the challenge of crystal structure prediction in the dicult case of the repeatedly studied, abundantly used aminoacid glycine that hosts still little-known phase transitions [14, 75, 76] and illustrate the current state of the eld through this example. First, we introduce glycine polymorphs and describe the method used in this study. By using clustering technique, the result of evolutionary algorithm is analyzed. We identify all experimentally known structures of glycine as well as the hitherto unresolved ζ phase. The challenge in exploring a polymorphic

landscape is exposed in the case of α-glycine. We suggest a simple way to explore

the energy-landscape more eciently. Finally, we propose several new low-energy structures of glycine.

### 3.1 Introduction

Glycine, H3N+CH2COO− as shown in Fig. 3.1(a), the smallest aminoacid, is an

excellent test case for organic crystal structure prediction studies as its already rich polymorphism under ambient conditions is amplied and becomes less understood at higher pressure (see Fig. 3.1 (b)). At ambient conditions, three polymorphs of glycine are known: α, β, and γ. The form readily obtained by evaporation of

aqueous solutions is α-glycine, which for long was believed to be the most stable

phase instead of the later discovered ground-state phase γ. However, the energy

dierence between the two phases is pretty small, about 0.27 kJ/mol per molecule [77]. Theγ-form appears if the crystallization is performed in acidied solutions [78]

Figure 3.1: (a) Glycine molecule with numbering of the atoms; (b) Glycine poly-morphism under pressure. Stability order of polymorphs at ambient pressure , α, β,γ with indicated Z molecules in unit cell, is given. When the pressure increases,

while phases β and γ transform into phases δ and ε respectively, α-glycine is still

stable up to at least 23 GPa. The ζ-glycine is formed on decompression of phaseε

at 0.62 GPa. However its crystal structure has not been resolved yet.

or by using compounds that prevent the growth of α-glycine [79]. β-glycine can be

obtained in the crystallization from aqueous solution with slow diusion of ethanol [80]. Nevertheless, it is unstable and usually transforms spontaneously into either

α or γ polymorphs [81].

Pressure evolution of ambient pressure phases shows that while γ and β phases

quickly lose single crystal nature or undergo a phase transition within a few GPa,

α phase stays stable up to 23 GPa, the highest pressure reached in experiments. A

reversible, hysteresis-free single-crystal to single-crystal transition occurs from β to δ phase at 0.76 GPa. Single crystals of the γ phase undergo instead an extended

polymorphic transformation in the wide range from 1.9 GPa to 7.6 GPa, to a high-pressure polymorph, the ε phase, accompanied with the fragmentation of single

3.2. Method 35 where a new, irreversible phase transition occurs to the ζ phase, a new polymorph

which is reported to be stable at ambient conditions for at least three days [14]. Interestingly, despite its stability, and at least three crystal structure prediction studies devoted to glycine so far [9, 60, 82], a decade after its observation, the ζ

phase has not been structurally resolved yet. In the study of the low-temperature heat capacity of β-glycine, a second order phase transition was observed at 252 K

[75]. However, the crystal structure of this newβ00 phase has not been reported so

far and its existence has even been dismissed in subsequent work of the same group. In Ref. [76], glycine phases were studied when aqueous solutions were frozen, then the subsequent heating under dierent conditions resulted in an unknown X-glycine at 209-216 K. As temperature increases, this phase quickly transforms into the β

-polymorph. The crystal structure of X-glycine is also not fully determined, the experimental and calculated diraction patterns do not entirely agree. Motivated by the unknown structures, we perform the crystal structure prediction for glycine to search for possible low-energy structures and illustrate the current state of the eld through this example.

### 3.2 Method

3.2.1 Evolutionary search

The complex polymorphism of glycine highlights the importance of performing an extensive search in phase space, while practical concerns limit any crystal structure prediction study to explore primarily the lowest energy structures. In this study, we use evolutionary algorithms as implemented in the USPEX package to address this interplay eciently [9]. We perform three test suits with Z=2, 3 or 4 glycine molecules in the crystal unit cell. At the rst generation, 30 structures are created randomly. After energy ordering, the 20% of the population that is energetically

least favorable is discarded. Among the remaining structures, a ngerprint analysis is performed and potential parents whose ngerprint is within a threshold distance of 0.01 from any lower energy structure are also discarded. The so-determined unique structures are eligible as parents and are allowed to procreate. The structures of the

new generation are created from parents through the following operations: heredity (cross-over of two structures) (40%), softmutation (translation and rotation based

on an estimate of soft vibrational modes) (20%) and rotation of the molecule (20%).

The diversity of the population is guaranteed by addition of new random structures (20%) at each generation, while the three best parents are directly cloned to the

next generation. The highest computational cost in this workow is due to the ab initio geometry optimization of each structure considered. To keep this cost well within the capacity of modern high-performance computing technologies and within the budget of academic as well as industrial research, we limit the evolution to 20 generations at most.

3.2.2 ab initio calculations

For every structure generated by USPEX, the geometry and cell relaxation is per-formed using vdW-DF functional [10,32] which was implemented in the QUANTUM ESPRESSO package [83]. A kinetic energy cuto of 80 Ryd and a charge density

cuto of 560 Ryd are used. The Brillouin zone sampling resolution was gradually

increased in three steps during relaxation: resolution of2π×0.12Å−1,2π×0.10Å−1

and 2π×0.08 Å−1 respectively. Energies and geometries of the last step with the

densest k-point are used throughout the study. PAW pseudopotentials are taken from the PSLibrary project [84]. By using this setup all structures are fully relaxed within a convergence of less than 0.1 mRy for absolute total energy, 0.5 mRy/a.u.

for the forces on atoms and less than 0.005GPa for the stress tensor.

3.2.3 Cluster analysis

A cluster analysis of the structures generated during the crystal structure prediction runs is performed by using single linkage clustering, where two structures with n-gerprint distance less than a distance threshold, d, are considered to belong to the same cluster. Since USPEX denition of ngerprint does not include any informa-tion on the enthalpy of the structure, a constraint is added such that two structures with enthalpy dierence more than 0.5 kJ/mol are not allowed to form a cluster.

3.3. Results 37 This constraint is found necessary only when the clustering analysis is performed for all the encountered structures, while when limiting the analysis to the low enthalpy region, such constraint was not necessary as each cluster was successfully identied with the distance only.

### 3.3 Results

3.3.1 Performances of several van der Waals functionals

First, we show the results of several van der Waals functionals to the structural and energetic properties of the three known polymorphs of glycine that are stable at ambient pressure. Four functionals are chosen in this study: the vdW-DF functional with revPBE for exchange part [32]; the rVV10 functional [37] which is the revised version of the VV10 functional [11] with the optimized parameterb= 6.3; the rVV10

functional with a modied parameter b = 9.3 as suggested in [38]; and the

semi-empirical PBE+D one [28]. We use the notation rVV10-b6.3 and rVV10-b9.3 to

indicate the rVV10 functional with the parameterbset to 6.3 and 9.3, respectively.

Table 3.1shows the optimized lattice parameters at zero pressure for α,β and γ phases with the four van der Waals functionals. The experimental lattice

pa-rameters of these structures, are also given. The PBE+D and rVV10-b6.3 give the

best descriptions of the cell parameters; changing parameter b to 9.3 makes the

rVV10-b9.3 give slightly worse cell parameters than rVV10-b6.3; while vdW-DF too

overestimates the cell parameters.

Next, we study the performance of these functionals in reproducing the structure of the single molecules in the crystal. In Table 3.2, we compare the bond lengths and torsion angle for α-glycine at ambient pressure. Changing parameter b from

6.3 to 9.3 of rVV10 functional doesn't make any eect in terms of bond lengths. The rVV10-b6.3, rVV10-b9.3 and PBE+D give very good values for bond lengths

while vdW-DF again overestimates the bond lengths, especially the C1-C2 and C2-N bonds. In terms of torsion angles, PBE+D and rVV10-b6.3 give the best comparisons

with experiment while vdW-DF and rVV10-b9.3 overestimate these angles.

poly-Table 3.1 Optimized cell parameters and the unit cell volume per moleculeV0 (Å 3

) at zero pressure for glycine phases that are stable at ambient pressure. The results are shown for dierent van der Waals functionals and the experimental data are also given. a (Å) b (Å) c (Å) β (deg) V0 α-glycine Exp.[85](77K) 5.069 11.801 5.448 111.7 75.70 vdW-DF 5.240 12.283 5.565 111.1 83.73 rVV10-b6.3 5.113 11.695 5.500 111.3 76.68 rVV10-b9.3 5.144 11.856 5.510 110.7 78.54 PBE+D 5.053 11.778 5.465 112.6 75.10 β-glycine Exp.[85](77K) 5.077 6.145 5.374 113.2 77.05 vdW-DF 5.212 6.409 5.500 112.4 84.74 rVV10-b6.3 5.091 6.119 5.437 113.3 76.68 rVV10-b9.3 5.117 6.210 5.439 112.6 79.77 PBE+D 5.039 6.107 5.406 113.8 76.11 γ-glycine Exp.[85](77K) 6.985 6.985 5.483 90.0 76.87 vdW-DF 7.233 7.232 5.587 90.0 84.34 rVV10-b6.3 6.985 6.986 5.523 90.0 77.82 rVV10-b9.3 7.057 7.057 5.540 90.0 79.65 PBE+D 6.919 6.919 5.491 90.0 75.87

3.3. Results 39 Table 3.2 Optimized bond lengths (Å) and torsion angle (degree) forα-glycine at

zero pressure. The results are shown for dierent van der Waals functionals and the experimental data are also given.

Bonds Exp.[85] vdW-DF rVV10-b6.3 rVV10-b9.3 PBE+D

C1-O1 1.25 1.27 1.27 1.27 1.26 C1-O2 1.25 1.27 1.27 1.27 1.27 C2-N 1.48 1.51 1.49 1.49 1.48 C1-C2 1.52 1.55 1.53 1.53 1.53 C2-H1 1.05 1.09 1.10 1.10 1.10 C2-H2 1.04 1.09 1.09 1.09 1.10 N-H3 1.03 1.04 1.05 1.05 1.05 N-H4 1.09 1.06 1.06 1.06 1.06 N-H5 1.09 1.03 1.04 1.04 1.04 Torsion N-C2-C1-O1 18.6 23.1 22.5 23.2 22.5

Table 3.3 Relative energies (in kcal/mol per molecule) for the glycine polymorphs at zero pressure. The results are shown for dierent van der Waals functionals and the experimental data are also given.

Functionals α β γ Exp. [77] 0.064 0.142 0 vdW-DF 0.016 0.264 0 rVV10-b6.3 -0.107 0.295 0 rVV10-b9.3 0.013 0.231 0 PBE+D 0.223 0.758 0

morphs at ambient pressure and the pressure values for theβ-δ andγ-εphase

tran-sitions. As seen in Table3.3, rVV10-b6.3 predicts a wrong energy ordering between α and γ phases; PBE+D gives right stability ordering, but the energy dierences

are too much overestimated; vdW-DF and rVV10-b9.3 are the ones which agree very

phase transitions from β to δ and fromγ to ε occur experimentally and those

pre-dicted by van der Waals functionals. While rVV10-b6.3 (PBE+D) underestimates

(overestimates) these pressure values; vdW-DF and rVV10-b9.3 agree very well with

experiment.

Among the functionals used in this study, we show that the ones that give a better description of the structural properties, give worse results for the energetic properties and vice versa. These results show that signicant room for improvement of the van der Waals functionals still remains. For crystal structure prediction, the energy ordering is the most important aspect, therefore we choose to use the vdW-DF functional.

Table 3.4 The pressure phase transitions (in GPa) from β-δ and γ-ε of glycine

polymorphs. The results are shown for dierent van der Waals functionals, and the experimental data are also given.

Phase transition Exp. vdW-DF rVV10-b6.3 rVV10-b9.3 PBE+D β-δ 0.76 [86] 1.5 0.15 1.1 1.25 γ-ε 1.90 [87] 1.8 1.00 1.8 2.54

3.3.2 Results of evolutionary algorithm

The results of crystal structure prediction can be visualized through the distribu-tion of energy as a funcdistribu-tion of volume for the structures encountered during the search. Despite the exploration of a wide region in phase space (see left panel of Fig.3.2), about 40 % of all the structures lies within 4 kJ/mol of the experimentally known ground state structure, γ. Focusing on this region of the energy-landscape

as shown in the right panels of Fig.3.2, we see structures forming islands with vary-ing sizes and shapes. This feature illustrates the added complication in the case of molecular crystal structure prediction with respect to standard inorganic solids where well-dened, isolated minima would be observed for each phase. The shape and nite size of the islands can be understood considering that Glycine is very soft, therefore structures that are far o from the equilibrium lattice parameters are thermodynamically penalized only slightly as demonstrated in the inset of Fig.3.2.

3.3. Results 41

Figure 3.2: Results of ab initio crystal structure search for Glycine with cluster analysis. Left panel: Enthalpy vs volume distribution of all encountered structures for 2 molecules per cell shows that CSP with evolutionary algorithm al-lows a wide energy range to be explored while survival of the ttest algorithm keeps the focus on the thermodynamically low lying structures. Right panels: Ex-panded view of all explored structures compatible with 2, 3 and 4 molecules per cell in the lowest 4 kJ/mol range. All known phases of glycine are identied with the right energy ordering along with a number of low-lying alternative polymorphs, including our prediction for the hitherto unresolved ζ phase. As shown in the inset

of the Z=4 panel, crowding around each polymorph, when compared with its equa-tion of state, is compatible with numerical noise due to incomplete relaxaequa-tion. The ngerprint-and-energy based clustering techniques adopted here are however well suited to separate and identify the dierent low lying polymorphs even in presence of noise.

This eect, combined with the numerical noise in geometry optimization, as well as an increased number of degrees of freedom in molecular crystals, is enough to give rise to crowding around each polymorphic minimum. Nevertheless islands are well separated and a clear assignment of polymorphs can be made for most of them. This is in stark contradiction with a very recent crystal structure prediction study

for glycine with empirical corrections for intermolecular interactions, which reported that the obtained energy-volume points were not well separated enough to clearly identify each polymorph, thus underlining the challenge of polymorphism for or-ganic crystal structure prediction [60]. In this study instead the separation between several islands are well represented down to very small energy dierences (inset of Fig.3.2). We believe this stems from the leap in accuracy and precision reached by the use of fully ab initio energetics together with last generation evolutionary algorithm tools.

3.3.3 Clustering algorithm

Reliable energetics from ab initio calculations is necessary but not sucient to guar-antee a reliable structure classication in crystal structure prediction. More than one polymorph can be present within a given extended island; or what appears to be two adjacent islands due to insucient sampling and/or relaxation, may actually correspond to the same packing order. Indeed the most human-time consuming part of a crystal structure prediction procedure is known to be the stage where the output structures are comparatively examined in order to successfully separate the essen-tial data from the crowd of repetitions [1]. Although not utilized to their full extent within crystal structure prediction, concepts from data mining, mainly clustering techniques, can be of great help in this stage of the analysis, as we demonstrate in the following.

We used the clustering technique to identify the unique polymorphs among all the structures obtained with crystal structure prediction. In this clustering analy-sis, a bottom-up distance-based hierarchical clustering approach with single linkage is used. In distance-based approaches, a similarity metric is dened so that a dis-tance can be measured between data points, and clusters are constructed based on proximity.

3.3. Results 43

Figure 3.3: The number of clusters as a function of the distance threshold,d, for all

structures (green curve) and low-energy structures within approximately 4 kJ/mol above the ground state (blue curve) for the case ofZ = 2. Insets show the enthalpy

(kJ/mol) as a function of volume (Å3

) per molecule for dierent values of d = 0.01, 0.08, 0.2, 0.35. Dierent colors and point types in each inset correspond to

dierent clusters. The value of d = 0.052−0.10 can distinguish dierent clusters

Figure 3.4: The number of clusters as a function of the distance threshold, d, for all

structures (green curve) and low-energy structures within approximately 4 kJ/mol above the ground state (blue curve) for the case ofZ = 3. Insets show the enthalpy

(kJ/mol) as a function of volume (Å3

) per molecule for dierent values of d = 0.01, 0.08, 0.15, 0.25. Dierent colors and point types in each inset correspond to

dierent clusters. The value of d = 0.05−0.09 can distinguish dierent clusters

3.3. Results 45

Figure 3.5: The number of clusters as a function of the distance threshold,d, for all

structures (green curve) and low-energy structures within approximately 4 kJ/mol above the ground state (blue curve) for the case ofZ = 4. Insets show the enthalpy

(kJ/mol) as a function of volume (Å3

) per molecule for dierent values of d = 0.01, 0.08, 0.2, 0.26. Dierent colors and point types in each inset correspond to

dierent clusters. The value of d = 0.07−0.09 can distinguish dierent clusters

In this study we use as the metric, the ngerprint-based cosine distance [9,69,70] dened in the evolutionary algorithm code USPEX [13]:

Dcosine(µ, ν) = 1 2 1− Fµ∗Fν |Fµ| |Fν| , (3.1)

where individual structure ngerprints are dened as

FAB(R) =
X
Ai,cell
X
Bj
δ(R−Rij)
4πR2_{ij}NANB_{V} ∆−1, (3.2)

where the double sum runs over allith molecules of typeAwithin the unit cell and

alljth molecules of typeB within a distanceRmax;δ(R−Rij)is a Gaussian-smeared delta function; Rij is the distance measured from the centers of molecules i and j;

V is the unit cell volume; the function FAB(R)is discretized over bins of width ∆;

NAand NB are the numbers of molecules of type A andB, respectively.

In Figs. 3.3, 3.4 and 3.5, we display a step by step clustering analysis in the cases Z = 2, 3, 4 respectively. In these gures, the green (blue) curve is for the case in which the whole data set (the low-energy structures within 4.2 kJ/mol of the ground state) are considered. The distance threshold used to dene whether two data points belong to the same cluster is then monotonically increased. As a result the cluster population evolves from the situation where every data point forms a distinct cluster to the situation in which all data points belong to the same global cluster, revealing the bottom-up and hierarchical nature of the approach. The most impressive feature of these gures is that the behavior of a rapid drop in the number of clusters is followed by a more or less constant plateau before the number of clusters eventually dies o. This behavior is quite general and applies to all cases of Z = 2, 3, 4 and when the whole data set or low-energy structures are considered. Translated to the crystal structure prediction problem, this data mining approach transforms the challenge of identication of unique polymorphs from the visual comparison of all structures into an easier decision on the value of the distance-threshold to be adopted. The optimal distance threshold is such that each data cluster matches a unique physical polymorph. In the case of glycine a distance threshold around 0.08 is found to be appropriate to identify the low energy polymorphs successfully. The so-determined optimal threshold can serve in advanced supervised learning

3.3. Results 47

Figure 3.6: a. Comparison of simulated x-ray diraction patterns for ε-, γ- and ζ

- glycine at 2 GPa with experimental data taken from [14] at 0.2 GPa. The XRD of proposed ζ-glycine can explain most of the unassigned peaks that were marked

in the experimental spectrum, especially the ones highlighted in the purple boxes. The theoretical data is calculated at higher pressure to oset the overestimation of the ground state volume in ab initio calculations. b. Enthalpy per molecule as a function of pressure for ε-glycine and ζ-glycine with respect to the γ phase up to 5

GPa. The black arrows indicate the phase transitions observed in the experiment [14]: Under pressure, the γ phase undergoes a phase transition to ε-glycine. The

decompression ofε-glycine instead results in theζ phase.

techniques and be fed back in the crystal structure prediction procedure to increase considerably the eciency by reducing the generation of replicas of already explored structures.

3.3.4 Identication of ζ-glycine

The cluster analysis outlined above identies all experimentally observed phases of glycine compatible with 2, 3 or 4 molecules per cell, as well as suggests